1 PROJECT REPORT OnAnalyze submerged arc welding(SAW) with respect to MIG welding(GMAW) Project guide: Mr. AAYUSH SINGHAL (Asst. Manager, QA) SUBMITTED BY: NISHANT RAO BODDEDA B.TECH MECHANICAL ENGINEERING K.L UNIVERSITY VADDESSWARAM,GUNTUR DISTRICT
2 INDEXSL.NO. CONTENTS Page no. 1 Acknowledgement 3 2 Certificate 4 3 Objective 5 Introduction to 4 6 welding 5 Classification 7 6 8 Introduction to SAW 7 Principle of operation, 9 Equipments 8 SAW welding in 20 telcon, advantages and its limitations 9 Introduction to MIG 28 or GMAW. Various parameters, 30 10 operations ,difference between SAW and GMAW Advantages, limitations and 11 conclusion 33
3 ACKNOWLEDGEMENTAt the cynosure of my voyage I wish to take this opportunity to express myineffable sense of profound gratitude to Mr. Kumar Jagat (Manager-HR,TELCON) for giving me this golden opportunity to be a part of this renownedorganization as a summer trainee.Furthermore I wholeheartedly, acknowledge the intellectual simulation of myesteemed guide Mr.Somnath nayak (Sr.Manager-QA) and Mr.Aayushsinghal(Assistant manager-QA) for his valuable guidance and the motivationthat made my project a real success in spite of their hectic schedule.I am deeply indebted to all the officers for their expert suggestions during thetenure of this project work.I am highly grateful to all the operators and the support staff for their help inevery aspect during this period.Finally, my sincere regards to my parents, relatives and all my friends whohave been a constant source of encouragement and moral support allthroughout.PLACE:TELCON, JAMSHEDPUR
4 CERTIFICATE THIS IS TO CERTIFY THAT NISHANT RAOBODDEDA BEARING ID NO. 10101812 PURSUINGBACHELOR OF ENGINEERING IN THE STREAM OFMECHANICAL IN K.L UNIVERSITY,VADDESSWARAM, GUNTUR DISTRICT HASSUCESSFULLY COMPLETED TRAINING IN TELCOCONSTRUCTION AND EQUIPMENT COMPANYLTD. FROM 14-05-2012 , HAS DONE A PROJECTIN “Analyze submerged arc welding(SAW) withrespect to MIG welding (GMAW)”.
5AIM: To have a comparative study of submerged arcwelding(SAW) with respect to MIG welding (GMAW).OBJECTIVE:1. To study the submerged arc welding and MIG welding.2. To learn about all the various parameters in the process.3. To do comparative analysis between SAW and GMAW.4. Various products manufactured by this processes.5. Recommended corrective actions can be taken.Rationale of the study:1. To know about the widest range of welding processes taking place on TELCON2. To improve the quality by minimizing the defects occurs, during welding3. To study about the various construction equipments in telcon.
6Expected contribution from the study:1. Improvement in quality2. Less defects per job3. Maximum productivity in less time WELDINGINTRODUCTION:Welding is a materials joining process which produces coalescence ofmaterials by heating them to suitable temperatures with or without theapplication of pressure or by the application of pressure alone, and with orwithout the use of filler material.Welding is used for making permanent joints.It is used in the manufacture of automobile bodies, aircraft frames, railwaywagons, machine frames, structural works, tanks, furniture, boilers, generalrepair work and ship building.
8 SUBMERGED ARC WELDING(SAW)INTRODUCTION:Submerged arc welding is a process in which the joiningof metals is produced by heating with an arc or arcsbetween a bare metal electrode or electrodes and thework. The arc is shielded by a blanket of granular fusiblematerial on the work. Pressure is not used. Filler metal isobtained from the electrode or from a supplementarywelding rod.
9EQUIPMENT: (1) The equipment components required for submerged arc welding are shown by figure 10-59. Equipment consists of a welding machine or power source, the wire feeder and control system, the welding torch for automatic welding or the welding gun and cable assembly for semiautomatic welding, the flux hopper and feeding mechanism, usually a flux recovery system, and a travel mechanism for automatic welding.
10(2) The power source for submerged arc welding must be rated for a 100 percentduty cycle, since the submerged arc welding operations are continuous and thelength of time for making a weld may exceed 10 minutes. If a 60 percent duty cyclepower source is used, it must be derated according to the duty cycle curve for 100percent operation.(3) When constant current is used, either ac or dc, the voltage sensing electrodewire feeder system must be used. When constant voltage is used, the simpler fixedspeed wire feeder system is used. The CV system is only used with direct current.(4) Both generator and transformer-rectifier power sources are used, but the rectifiermachines are more popular. Welding machines for submerged arc welding range insize from 300 amperes to 1500 amperes. They may be connected in parallel toprovide extra power for high-current applications. Direct current power is used forsemiautomatic applications, but alternating current power is used primarily with themachine or the automatic method. Multiple electrode systems require specializedtypes of circuits, especially when ac is employed.(5) For semiautomatic application, a welding gun and cable assembly are used tocarry the electrode and current and to provide the flux at the arc. A small fluxhopper is attached to the end of the cable assembly. The electrode wire is fedthrough the bottom of this flux hopper through a current pickup tip to the arc. Theflux is fed from the hopper to the welding area by means of gravity. The amount offlux fed depends on how high the gun is held above the work. The hopper gun mayinclude a start switch to initiate the weld or it may utilize a "hot" electrode so thatwhen the electrode is touched to the work, feeding will begin automatically.(6) For automatic welding, the torch is attached to the wire feed motor and includescurrent pickup tips for transmitting the welding current to the electrode wire. The
11 flux hopper is normally attached to the torch, and may have magnetically operated valves which can be opened or closed by the control system. (7) Other pieces of equipment sometimes used may include a travel carriage, which can be a simple tractor or a complex moving specialized fixture. A flux recovery unit is normally provided to collect the unused submerged arc flux and return it to the supply hopper. (8) Submerged arc welding system can become quite complex by incorporating additional devices such as seam followers, weavers, and work rovers.Principles of Operation. (1) The submerged arc welding process is shown by figure 10-60. It utilizes the heat of an arc between a continuously fed electrode and the work. The heat of the arc melts the surface of the base metal and the end of the electrode. The metal melted off the electrode is transferred through the arc to the workpiece, where it becomes the deposited weld metal. Shielding is obtained from a blanket of granular flux, which is laid directly over the weld area. The flux close to the arc melts and intermixes with the molten weld metal, helping to purify and fortify it. The flux forms a glass-like slag that is lighter in weight than the deposited weld metal and floats on the surface as a protective cover. The weld is submerged under this layer of flux and slag, hence the name submerged arc welding. The flux and slag normally cover the arc so that it is not visible. The unmelted portion of the flux can be reused. The electrode is fed into the arc automatically from a coil. The arc is maintained automatically. Travel can be manual or by machine. The arc is initiated by a fuse type start or by a reversing or retrack system. (2) Normal method of application and position capabilities. The most popular method of application is the machine method, where the operator monitors the welding operation. Second in popularity is the automatic method, where welding is a pushbutton operation. The process can be applied semiautomatically; however, this method of application is not too popular. The process cannot be applied manually because it is impossible for a welder to control an arc that is not visible. The submerged arc welding process is a limited-position welding process. The welding positions are limited because the large pool of molten metal and the slag are very fluid and will tend to run out of the joint. Welding can be done in the flat position and in the horizontal fillet position with ease. Under special controlled procedures, it is possible to weld in the horizontal position, sometimes called 3 oclock welding. This
12requires special devices to hold the flux up so that the molten slag and weld metalcannot run away. The process cannot be used in the vertical or overhead position.(3) Metals weldable and thickness range. Submerged arc welding is used to weldlow- and medium-carbon steels, low-alloy high-strength steels, quenched andtempered steels, and many stainless steels. Experimentally, it has been used to weldcertain copper alloys, nickel alloys, and even uranium. This information issummarized in table 10-21.Metal thicknesses from 1/16 to 1/2 in. (1.6 to 12.7 mm) can be welded with no edgepreparation. With edge preparation, welds can be made with a single pass onmaterial from 1/4 to 1 in. (6.4 to 25.4 mm). When multipass technique is used, themaximum thickness is practically unlimited. This information is summarized in table10-22. Horizontal fillet welds can be made up to 3/8 in. (9.5 mm) in a single passand in the flat position, fillet welds can be made up to 1 in. (25 mm) size.(4) Joint design. Although the submerged arc welding process can utilize the samejoint design details as the shielded metal arc welding process, different joint detailsare suggested for maximum utilization and efficiency of submerged arc welding. Forgroove welds, the square groove design can be used up to 5/8 in. (16 mm)thickness. Beyond this thickness, bevels are required. Open roots are used butbacking bars are necessary since the molten metal will run through the joint. Whenwelding thicker metal, if a sufficiently large root face is used, the backing bar may beeliminate. However, to assure full penetration when welding from one side, backingbars are recommended. Where both sides are accessible, a backing weld can be
13made which will fuse into the original weld to provide full penetration. Recommendedsubmerged arc joint designs are shown by figure 10-61 below.
14(5) Welding circuit and current. (a) The welding circuit employed for single electrode submerged arc welding is shown by figure 10-59. This requires a wire feeder system and a power supply. (b) The submerged arc welding process uses either direct or alternating current for welding power. Direct current is used for most applications which use a single arc. Both direct current electrode positive (DCEP) and electrode negative (DCEN) are used. (c) The constant voltage type of direct current power is more popular for submerged arc welding with 1/8 in. (3.2 mm) and smaller diameter electrode wires. (d) The constant current power system is normally used for welding with 5/3 2 in. (4 mm) and larger-diameter electrode wires. The control circuit for CC power is more complex since it attempts to duplicate the actions of the welder to retain a specific arc length. The wire feed system must sense the voltage across the arc and feed the electrode wire into the arc to maintain this voltage. As conditions change, the wire feed must slow down or speed up to maintain the prefixed voltage across the arc. This adds complexity to the control system. The system cannot react instantaneously. Arc starting is more complicated with the constant current system since it requires the use of a reversing system to strike the arc, retract, and then maintain the preset arc voltage. (e) For ac welding, the constant current power is always used. When multiple electrode wire systems are used with both ac and dc arcs, the constant current power system is utilized. The constant voltage system, however, can be applied when two wires are fed into the arc supplied by a single power source. Welding current for submerged arc welding can vary from as low as 50 amperes to as high as 2000 amperes. Most submerged arc welding is done in the range of 200 to 1200 amperes.(6) Deposition rates and weld quality. (a) The deposition rates of the submerged arc welding process are higher than any other arc welding process. Deposition rates for single electrodes are shown by figure 10-62. There are at least four related factors that control the deposition rate of submerged arc welding: polarity, long stickout, additives in the flux, and additional electrodes. The deposition rate is the highest for direct current electrode negative (DCEN). The deposition rate for alternating current is between DCEP and DCEN. The polarity of maximum heat is the negative pole.
15(b) The deposition rate with any welding current can be increased byextending the "stickout." This is the distance from the point where current isintroduced into the electrode to the arc. When using "long stickout" theamount of penetration is reduced. The deposition rates can be increased bymetal additives in the submerged arc flux. Additional electrodes can be usedto increase the overall deposition rate.(c) The quality of the weld metal deposited by the submerged arc weldingprocess is high. The weld metal strength and ductility exceeds that of the mildsteel or low-alloy base material when the correct combination of electrodewire and submerged arc flux is used. When submerged arc welds are made bymachine or automatically, the human factor inherent to the manual weldingprocesses is eliminated. The weld will be more uniform and free frominconsistencies. In general, the weld bead size per pass is much greater withsubmerged arc welding than with any of the other arc welding processes. Theheat input is higher and cooling rates are slower. For this reason, gases areallowed more time to escape. Additionally, since the submerged arc slag islower in density than the weld metal, it will float out to the top of the weld.Uniformity and consistency are advantages of this process when appliedautomatically.(d) Several problems may occur when using the semiautomatic applicationmethod. The electrode wire may be curved when it leaves the nozzle of thewelding gun. This curvature can cause the arc to be struck in a location notexpected by the welder. When welding in fairly deep grooves, the curvaturemay cause the arc to be against one side of the weld joint rather than at theroot. This will cause incomplete root fusion. Flux will be trapped at the root ofthe weld. Another problem with semiautomatic welding is that of completelyfilling the weld groove or maintaining exact size, since the weld is hidden andcannot be observed while it is being made. This requires making an extrapass. In some cases, too much weld is deposited. Variations in root opening
16 affect the travel speed. If travel speed is uniform, the weld may be under- or overfilled in different areas. High operator skill will overcome this problem. (e) There is another quality problem associated with extremely large single- pass weld deposits. When these large welds solidify, the impurities in the melted base metal and in the weld metal all collect at the last point to freeze, which is the centerline of the weld. If there is sufficient restraint and enough impurities are collected at this point, centerline cracking may occur. This can happen when making large single-pass flat fillet welds if the base metal plates are 45° from flat. A simple solution is to avoid placing the parts at a true 45° angle. It should be varied approximately 10° so that the root of the joint is not in line with the centerline of the fillet weld. Another solution is to make multiple passes rather than attempting to make a large weld in a single pass. (f) Another quality problem has to do with the hardness of the deposited weld metal. Excessively hard weld deposits contribute to cracking of the weld during fabrication or during service. A maximum hardness level of 225 Brinell is recommended. The reason for the hard weld in carbon and low-alloy steels is too rapid cooling, inadequate postweld treatment, or excessive alloy pickup in the weld metal. Excessive alloy pickup is due to selecting an electrode that has too much alloy, selecting a flux that introduces too much alloy into the weld, or the use of excessively high welding voltages. (g) In automatic and machine welding, defects may occur at the start or at the end of the weld. The best solution is to use runout tabs so that starts and stops will be on the tabs rather than on the product.(7) Weld schedules. The submerged arc welding process applied by machine or fullyautomatically should be done in accordance with welding procedure schedules. Table10-23 and figure 10-63, below, show the recommended welding schedules forsubmerged arc welding using a single electrode on mild and low-alloy steels. Thetable can be used for welding other ferrous materials, but was developed for mildsteel. All of the welds made by this procedure should pass qualification, tests,assuming that the correct electrode and flux have been selected. If the schedules arevaried more than 10 percent, qualification tests should be performed to determinethe weld quality.
20 (8) Welding variables. (a) The welding variables for submerged weld joint size and the current recommended for the particular joint. This must also be considered in determining the number of passes or beads for a particular joint. Welds for the same joint dimension can be made in many or few passes, depending on the weld metal metallurgy desired. Multiple passes usually deposit higher-quality weld metal. Polarity is established initially and is based on whether arc welding are similar to the other arc welding processes, with several exceptions. (b) In submerged arc welding, the electrode type and the flux type are usually based on the mechanical properties required by the weld. The electrode and flux combination selection is based on table 10-24, below, to match the metal being welded. The electrode size is related to the maximum penetration or maximum deposition rate is required.SUBMERGED ARC WELDING IN TELCON:Basically submerged arc welding is done for axle assembly.Process: It is a continuous process where filler material fills up the groove space by themelting of the electrode and continuous deposition of flux over it.LAYOUT
21Pre-heating stage: Heating is done upto temperature of 250degrees.Workers performing GOGGING operation:
22GROOVE MEASUREMENTS:The groove thickness is 3/8 inches and the groove length is of30mm .Taper angle is approximately 80 degrees.
23WORKER PERFORMING GRINDING WHEEL OPERATION:Grinding wheel grit size is 36.Functions of Electrodes Coating: • Provide a protective , non oxidizing or reducing gas shield around the arc to keep oxygen and nitrogen in the air away from molten metals. • Facilitates striking the arc and enables it to be stable • Provides flux for the molten pool of metal , forms a protective slag which is easily removed
24Types of flux/electrode:INCOFLUX NT100 Submerged Arc Flux is a neutral, agglomerated flux designed for wire welding with Nickel FillerMetal 61, INCONEL Filler Metals 82 and 625, NI-ROD 44 Filler Metal and NILO Filler Metals CF36 and CF42.Typical applications are groove welding Nickel 200 alloy to itself and to steels, and overlaying carbon steels with theNickel 61 filler metal. The flux is also suitable to use with INCONEL Filler Metals 82 and 625 for overlaying and multi-pass welding. NI-ROD 44 Filler Metal and INCOFLUX NT100 are used to submerged arc weld cast irons tothemselves and to steels. INCOFLUX NT100 is also used with NILO Filler Metal CF36 and CF42 to join Invar, NILO36 and NILO 42. Extension Stick- FluxDiameter Amperes Volts Travel Speed out DepthNickel 61 250-280 28-30 10-12 in / min 7/8-1 in 1/2-1 in0.062 in 250-305 mm / 22-25 mm 19-25 mm1.6 mm min0.093 in 250-300 30-33 8-11 in / min 7/8-1 in 3/4-1 1/42.4 mm 200-280 mm / 22-25 mm in min 19-32 mmWelding Parameters:Groove and Overlay Welding using DCEP current and Stringer beads.Overlay Welding with Oscillation:Use DCEN current and Oscillation Frequency of 50-70 cycles / min for 0.062 in. and 35-50 for 0.093 in.
25SpecificationEN 760 – S A AF2Particle SizeTyler Sieves: 10 x 60 Mesh (0.25 mm x 2.0 mm), EN 760 2-20. Advantages and Major Uses. (1) The major advantages of the submerged arc welding process are: (a) high quality of the weld metal. (b) extremely high deposition rate and speed. (c) smooth, uniform finished weld with no spatter. (d) little or no smoke. (e) no arc flash, thus minimal need for protective clothing. (f) high utilization of electrode wire. (g) easy automation for high-operator factor. (h) normally, no involvement of manipulative skills. (2) The submerged arc process is widely used in heavy steel plate fabrication work. This includes the welding of structural shapes, the longitudinal seam of larger diameter pipe, the manufacture of machine components for all types of heavy industry, and the manufacture of vessels and tanks for pressure and storage use. It is widely used in the shipbuilding industry for splicing and fabricating subassemblies, and by many other industries where steels are used in medium to heavy thicknesses. It is also used for surfacing and buildup work, maintenance, and repair.. Limitations of the Process.
26 (1) A major limitation of submerged arc welding is its limitation of welding positions. The other limitation is that it is primarily used only to weld mild and low-alloy high-strength steels. (2) The high-heat input, slow-cooling cycle can be a problem when welding quenched and tempered steels. The heat input limitation of the steel in question must be strictly adhered to when using submerged arc welding. This may require the making of multipass welds where a single pass weld would be acceptable in mild steel. In some cases, the economic advantages may be reduced to the point where flux-cored arc welding or some other process should be considered. (3) In semiautomatic submerged arc welding, the inability to see the arc and puddle can be a disadvantage in reaching the root of a groove weld and properly filling or sizing. MIG or GAS METAL ARC WELDING(GMAW) It is an electric arc welding process which joins metals by heating them with an arc established between a continuous filler metal (consumable) electrode and the work. Shielding of the arc and molten weld pool is obtained entirely from an externally supplied gas or gas mixture both inert and reactive gases.GMAW Welding Operations: . The process can be applied to a wide variety of metals, both ferrous and non-ferrous. A relatedprocess, flux-cored arc welding (FCAW), uses similar equipment but uses wire consisting of a steelelectrode surrounding a powder fill material. This cored wire is more expensive than the standard solidwire and can generate fumes and/or slag, but it permits higher welding speed and greater metalpenetration.
27Gas metal arc welding (GMAW), sometimes referred to by its subtypes, metal inert gas (MIG) welding ormetal active gas (MAG) welding, is a semi-automatic or automatic arc welding process in which acontinuous and consumable wire electrode and a shielding gas are fed through a welding gun. A constantvoltage, direct current power source is most commonly used with GMAW, but constant current systems,as well as alternating current, can be used.Originally developed for welding aluminum and other non-ferrous materials in the 1940s, GMAW wassoon applied to steels because it allowed for lower welding time compared to other welding processes.The cost of inert gas limited its use in steels until several years later, when the use of semi-inert gasessuch as carbon dioxide became common. Further developments during the 1950s and 1960s gave theprocess more versatility and as a result, it became a highly used industrial process. Today, GMAW iscommonly used in industries such as the automobile industry, where it is preferred for its versatility andspeed. Unlike welding processes that do not employ a shielding gas, such as shielded metal arc welding, itis rarely used outdoors or in other areas of air volatility. A related process, flux cored arc welding, oftendoes not utilize a shielding gas, instead employing a hollow electrode wire that is filled with flux on theinside.
28 MIG Machine with Spool feeder:GUN used in GMAW:
29GMAW Weld Diagram:Welding type - MIG/MAG Gas used - Ar mixed 80% Ar, 18% co2, 2% o2Working temp. - 6500 FPolarity - work piece(-ve) -Electrode (+ve)Filler metal -CCMSTorch -Tandem torch -Wire speed (i) 15 m/min
30 (ii) 9 m/minWelding parameters:Differences between SAW and GMAW:It is a automatic electrode It is an electric arc welding
31feeding machine wherein the process which joins metals bytip of the electrode is heating them with an arcsubmerged into a granular flux established between awhich shields the arc and the continuous filler metalmolten metal. (consumable) electrode and the work.The high quality of the weld The deposition rate is slow asmetal and extremely high compared to SAW anddeposition rate and speed medium quality of weld can bemakes it a suitable process. done.Advantages of GMAW: Produced High quality welds & much faster than with SMAW and TIG welding. No flux is used no slag entrapment in the weld metal. Very little loss of alloying elements as the metal transfers across the arc and minor weld spatter is produced, and it is easily removed. Limitations of GMAW:
32 IT cannot be used in the vertical or overhead welding positions due to the high heat input and the fluidity of the weld puddle. Has complex equipment compared to equipment used for the shielded metal-arc welding process. THANK YOU